| ||Format||Pages||Price|| |
|8||$42.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$42.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$50.40||  ADD TO CART|
Significance and Use
This test method provides a standard laboratory procedure for measuring and comparing the burning rates of polymeric materials under specified controlled conditions.
The rate of burning is affected by such factors as density, direction of rise, and type and amount of surface treatments. The thickness of the finished specimens must also be taken into account. These factors must be considered in order to compare materials on the same basis.
In this procedure, the specimens are subjected to one or more specific sets of laboratory test conditions. If different test conditions are substituted or the end-use conditions are changed, it is not always possible by or from this test method to predict changes in the fire-test-response characteristics measured. Therefore, the results are valid only for the fire test exposure conditions described in this procedure.
1.1 This test method is intended for use as a small-scale laboratory procedure for comparing the relative horizontal burning rates of polymeric materials used in occupant compartments of motor vehicles.
1.2 Units—The values stated in SI units are to be regarded as standard.
1.3 This test method, Federal Safety Standard MVSS 302, SAE J369, and ISO 3795 address the same subject matter, but differ in technical content.
1.4 This standard is used to measure and describe the response of materials, products, or assemblies to heat and flame under controlled conditions, but does not by itself incorporate all factors required for fire hazards or fire risk assessment of materials, products, or assemblies under actual fire conditions.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Specific hazard statements are given in Section 7.
1.6 Fire testing is inherently hazardous. Adequate safeguards for personnel and property shall be employed in conducting these tests.
Note 1—This standard and ISO 3795 address the same subject matter, but differ in technical content.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D5025 Specification for Laboratory Burner Used for Small-Scale Burning Tests on Plastic Materials
E176 Terminology of Fire Standards
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
SAE StandardSAEJ369 Flammability of Polymeric Interior Materials - Horizontal Test Method Available from Society of Automotive Engineers (SAE), 400 Commonwealth Dr., Warrendale, PA 15096-0001.
ISO StandardISO3795 Road vehicles, and tractors and machinery for agriculture and forestry--Determination of burning behavior of interior materials Available from International Organization for Standardization (ISO), 1 rue de Varemb, Case postale 56, CH-1211, Geneva 20, Switzerland.
ICS Number Code 43.040.60 (Bodies and body components); 83.060 (Rubber); 83.100 (Cellular materials)
UNSPSC Code 13100000(Rubber and elastomers)